Synthesis, Characterization, and Electrochemical Properties of a Series of Sterically Varied Iron(II) Alkoxide Precursors and Their Resultant Nanoparticles
Timothy J. Boyle; Leigh Anna M. Ottley; Christopher A. Apblett; Constantine A. Stewart; Sarah M. Hoppe; Krista L. Hawthorne; Mark A. Rodriguez; Inorganic Chemistry 50 (2011) 6174–6182; doi:10.1021/ic200423m

data_4325487
_publ_section_title
;
 Synthesis, Characterization, and Electrochemical Properties of a Series
 of Sterically Varied Iron(II) Alkoxide Precursors and Their Resultant
 Nanoparticles
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6174
_journal_page_last               6182
_journal_paper_doi               10.1021/ic200423m
_journal_volume                  50
_journal_year                    2011
_chemical_formula_sum            'C29 H29 Fe N3 O2'
_chemical_formula_weight         507.40
_space_group_IT_number           70
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-F 2uv 2vw'
_symmetry_space_group_name_H-M   'F d d d :2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            16
_cell_length_a                   13.493(2)
_cell_length_b                   28.102(5)
_cell_length_c                   29.703(5)
_cell_measurement_temperature    173(2)
_cell_volume                     11263(3)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0559
_diffrn_reflns_av_sigmaI/netI    0.0292
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       31
_diffrn_reflns_limit_k_min       -31
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       -32
_diffrn_reflns_number            16503
_diffrn_reflns_theta_full        23.30
_diffrn_reflns_theta_max         23.30
_diffrn_reflns_theta_min         1.81
_exptl_absorpt_coefficient_mu    0.563
_exptl_absorpt_correction_T_max  0.909
_exptl_absorpt_correction_T_min  0.894
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.197
_exptl_crystal_description       irregular
_exptl_crystal_F_000             4256
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.17
_refine_diff_density_max         0.304
_refine_diff_density_min         -0.261
_refine_diff_density_rms         0.048
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.213
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     161
_refine_ls_number_reflns         2035
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.213
_refine_ls_R_factor_all          0.0690
_refine_ls_R_factor_gt           0.0587
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0518P)^2^+24.6030P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1237
_refine_ls_wR_factor_ref         0.1290
_reflns_number_gt                1788
_reflns_number_total             2035
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic200423m_si_001_01.cif
_cod_data_source_block           10fb222ss
_cod_original_sg_symbol_H-M      'F d d d'
_cod_database_code               4325487